Chapter 2Alkaline Membrane Fuel CellsRobert C.T. Slade, Jamie P. Kizewski, Simon D. Poynton,Rong Zeng, and John R. VarcoeGlossaryAEM Alkaline (anion) exchange membrane.AFC Alkaline fuel cellAMFC Alkaline membrane fuel cell (also known as APEMFC)DMFC Direct methanol fuel cellMEA Membrane electrode assemblyOCV Open circuit voltagePEM Proton-exchange membranePEMFC Proton-exchange membrane fuel cellQA Quaternary ammoniumRG-AEM Radiation-grafted alkaline (anion) exchange membraneDeﬁnitionThe disruptive approach of applying alkaline anion-exchange membranes (AEMs) inalkaline membrane fuel cells (AMFCs) potentially meets several of the challengesfacing other approaches to low temperature fuel cells, including the otherwise highcatalyst and fuel costs. Thus, the move to alkaline conditions at the electrodes opensthe potential use of a range of low cost non-precious-metal catalysts, as opposed toThis chapter was originally published as part of the Encyclopedia of Sustainability Scienceand Technology edited by Robert A. Meyers. DOI:10.1007/978-1-4419-0851-3R.C.T. Slade (*) • J.P. Kizewski • S.D. Poynton • R. Zeng • J.R. VarcoeDepartment of Chemistry, University of Surrey, Guildford GU2 7XH, UKe-mail: R.Slade@surrey.ac.ukK.-D. Kreuer (ed.), Fuel Cells: Selected Entries from the Encyclopedia 9of Sustainability Science and Technology, DOI 10.1007/978-1-4614-5785-5_2,# Springer Science+Business Media New York 2013
10 R.C.T. Slade et al.the otherwise necessary use of platinum-group-metal (PGM) based catalysts. Further,it becomes possible to consider hydrogen fuels containing substantial amounts ofimpurities, whereas an acidic membrane approach (that in proton exchange membranefuel cells, PEMFCs) requires high-purity gases and PGM catalysts.IntroductionThe ﬁrst entry in the AMFC area was published in 2005 , since when activity andinterest have continued to increase steeply internationally. Zeng and Varcoe haverecently reviewed the developing patent literature . Some researchers haverecently termed these systems HEMFCs, hydroxide exchange membrane fuelcells; that terminology is not fully appropriate in view of the complex hydroxide/hydrogen carbonate/carbonate equilibria that are present (even after handlingmembranes in air), inevitable in the use of air (containing CO2(g)) as source ofoxidant and also produced in the oxidation of methanol in direct methanol fuel cells(DMFCs). Another acronym applied to these systems, APEMFCs, is also poten-tially confusing, the ﬁrst three words of the full form then seemingly being “alkalineproton exchange” (following the very similar PEMFC acronym) but being readablealternatively as alkaline polymer electrolyte membrane fuel cells (possibly AEMFCwould be clearer). Alkaline fuel cells (AFCs, hydrogen-fuelled cells with an alkaline liquid electro-lyte such as KOH(aq)) are the best performing of all known conventional hydrogen–oxygen fuel cells operable at temperatures below 200 C. This is due to the facilekinetics at the cathode and at the anode; cheaper non-noble metal catalysts can beused (such as nickel and silver [3, 4]), reducing cost. McLean et al. gave comprehen-sive review of alkaline fuel cell technology . The associated fuel cell reactions bothfor a traditional AFC and also for an AMFC are: Anode: 2H2 þ 4OHÀ ! 4H2 O þ 4eÀ ðEa ¼ 0:83 V vs: SHE at 1 bar; 298:15 KÞ Cathode: O2 þ 2H2 O þ 4eÀ ! 4OHÀ ðEc ¼ 0:40 V vs: SHE at 1 bar; 298:15 KÞ Overall: 2H2 þ O2 ! 2H2 O ðEcell ¼ 1:23 V at 1 bar; 298:15 KÞ A major issue with traditional AFCs is that of electrolyte and electrode degradationcaused by the formation of carbonate/bicarbonate (CO32À/HCO3À) on reaction ofOHÀ ions with CO2 contamination in the oxidant gas stream [5–7]:
2 Alkaline Membrane Fuel Cells 11 Carbonate formation : CO2 þ 2OHÀ ! CO3 2À þ H2 O Bicarbonate formation : CO2 þ OHÀ ! HCO3 À The major cause of the degrading performance of AFCs is the consequent precipi-tation of metal carbonate crystals (most commonly Na2CO3 or K2CO3, depending onthe alkaline electrolyte used) in the electrolyte-ﬁlled pores of the electrodes, blockingpores and mechanically disrupting and destroying active layers. The cost of fuel cells still retards commercialization in most markets. AFCs arepromising on a cost basis mainly because cheap and relatively abundant non-plati-num-group metals (non-PGM) are viable catalysts, but are hindered by degradationdue to formation of precipitates as above. Catalyst electrokinetics (for fuel oxidationand oxygen reduction) are improved in alkaline, as opposed to acidic, conditions (theacid-stability criterion precludes the use of most non-PGM catalysts in PEMFCs). Thereplacement of the KOH(aq) electrolyte with an alkaline electrolyte membrane(AEM), to give AMFCs, retains the electrocatalytic advantages but introduces CO2tolerance (there being no mobile cations that could give carbonate/bicarbonateprecipitates) with the additional advantage of being an all-solid-state fuel cell (aswith PEMFCs – i.e., no seeping out of KOH(aq)). Additionally, thin (low electronicresistance) and easily stamped (cheap) metal mono/bipolar plates can be used, withreduced corrosion-derived problems at high pH (the cost of bipolar plates for PEMFCscan be as much as one third of the cost of the stacks themselves). A key and yet to beconvincingly met requirement is, however, the development of a dispersible alkalineionomer (sometimes termed an anionomer) to maximize ionic contact between thecatalyst reaction sites and the ion-conductive membranes. As in the case of AFCs,water is produced at anode and consumed at cathode in AMFCs (when fuelled withhydrogen and with four electron reduction of oxygen at the cathode), which isfundamentally different to what occurs in PEMFCs containing acidic electrolytes;this can cause high overpotentials at AMFC anodes, due to suspected ﬂooding . The use of an AEM as a solid electrolyte including no metal cations preventsprecipitation of carbonate/bicarbonate salts. (The electrolyte containing the cationicgroups is already a solid.) The carbonation process is quick even if the AEM has beenexposed to the air for only a short time [9, 10]. The conductivities of the AEMs inOHÀ form may have been underestimated because most studies to date have notdisclosed vigorous CO2 exclusion procedures during conductivity measurements. Ithas been hypothesized that OHÀ ion conductivities in AEMs can be estimated bymeasuring the ionic conductivities of HCO3À from AEMs and multiplying by 3.8. This carbonation process may not to be a serious problem due to an in situ “self-purging mechanism” because OHÀ anions are continuously generated at the cathodein AMFCs . AEMs are solid polymer electrolyte membranes that contain positive ionicgroups (typically quaternary ammonium (QA) functional groups such as poly-NMe3+) and mobile negatively charged anions. A widely quoted concern with
12 R.C.T. Slade et al.AEMs is membrane stability, especially at elevated temperatures [13, 14]. Thegeneral issues are:1. The diffusion coefﬁcients and mobilities of OHÀ anions are less than that of H+ in most media, and QA ionic groups are less dissociated than the typical sulfonic acid groups (pKa for sulfonic acid groups are typically À1 but for QA groups the related pKb values are around +4); there were concerns that AEMs would not possess adequate intrinsic ionic conductivities for application in fuel cells.2. The OHÀ anions are effective nucleophiles which potentially cause degradation via (a) a direct nucleophilic displacement and/or (b) a Hofmann elimination reaction when a b-hydrogen is present; methyl (ÀCH3) groups may also be displaced by OHÀ ions forming tertiary amines and methanol [13, 14]. If the AEMs contain good leaving groups (e.g., QA –NMe3+ groups) then the chemical stability of the AEMs might have been inadequate for use in fuel cells, particularly at elevated temperatures.3. Precursor anion-exchange membranes are generally submerged in aqueous NaOH/KOH solutions to exchange them to the OHÀ form AEM; the AEM must have the chemical stability to withstand this process. Despite this, over a decade ago, the stabilities of various benzyltrimethylammonium-based AEMs were found to be stable at up 75 C in NaOH(aq) at concentrations up to 6 mol dmÀ3 for several days . A major potential application of AMFCs is, however, as power sources for at ornear room temperature (as for PEMFCs), which means such degradation can beminimal. This entry considers the current understanding and application of AEMs inhydrogen-fuelled AMFCs and other fuel cell types employing AEMs. Figure 2.1enables comparison between hydrogen- or methanol-fuelled PEMFCs and AMFCs;the electrode reactions in a hydrogen-fuelled AMFC are discussed above. In contrastto PEMFCs, operation of an AMFC requires the presence of water as a reagent at thecathode (oxygen reduction reaction, ORR – to form OHÀ) and the product water isformed by the hydrogen oxidation reaction (HOR) at the anode (as opposed to beingformed at the cathode in PEMFCs). The entry begins with consideration of the mainclasses of AEMs.An Overview of Alkaline Anion-Exchange Membranes (AEMs)AEMs and alkaline ionomers (anionomers) are key to the successful implementa-tion of AMFCs. Anion-exchange membranes have, for a long time, been used asseparation membranes for seawater desalination, the recovery of metal ions fromwastewaters, electrodialysis and bio-separation processes, for example [16–26].These membranes may, however, not be stable or conductive enough to be appliedin AMFCs. AEMs used in early AMFC studies were reviewed in 2005  andincluded polybenzimidazole (PBI) doped with KOH, epichlorohydrin polymer
2 Alkaline Membrane Fuel Cells 13a b 6e− Load 6e− 6e− Load 6e− 3H2 or 3H2 or[CH3 OH + H2O] 3/ O 2 2 [CH3 OH ] 3/ O +3H O 2 2 2 6H+ 6OH− Cathode Cathode Anode Anode 6H2 or [CO2] [CO2 + 5H2O] 3H2O Proton-Exchange Membrane Alkaline Anion-Exchange Membrane [PEM] [AAEM]Fig. 2.1 A schematic presentation of (a) a proton-exchange membrane (PEMFC) and (b) analkaline membrane fuel cell (AMFC), both fuelled either with H2 gas or directly with methanol(DMFC mode). The stoichiometric ratios of reactants and products are shown in each casequaternized with 1,4–diazabicyclo[2,2,2]octane (DABCO) or quaternized with a 1:1ratio of DABCO and triethylamine, and commercial membranes such as AHA(Tokuyama Co, Japan), Morgane ADP (Solvey S.A.), Tosﬂex® SF–17 (Tosoh) and2259–60 (Pall RAI). Most of these fuel cells containing AEMs were, however, beingoperated in the presence of aqueous alkaline solutions (containing NaOH or KOH). In the UK (at the University of Surrey), several kinds of QA-containingradiation-grafted AEMs (RG-AEMs) based on poly(vinylidene ﬂuoride) PVDF[27–31], poly(tetraﬂuoroethylene–co– hexaﬂuoropropylene) FEP [27, 28, 32] andpoly(ethylene-co-tetraﬂuoroethylene) ETFE [32, 33], with good ion-exchangecapacities (IEC) and ionic conductivities and with sufﬁcient stabilities to test theproof of concept of using AEMs in fuel cells, have been developed. ETFE baseﬁlms produce the best AEMs for testing in AMFCs. The radiation-grafted method-ology (using gamma rays or electron beams for irradiation) allowed for the produc-tion of AEMs of different thicknesses, ion-exchange capacity, physical/mechanicalproperties, and chemistries that facilitated fundamental investigations. A water-insoluble alkaline ionomer that used N,N,N’,N’–tetramethylhexane–1,6–diamine asthe joint amination and cross-linking agent ﬁrst enabled studies of the performanceof metal-cation-free all-solid-state alkaline fuel cells with stable performance intothe medium term at 50 C [33, 34]. Many other groups have now developed newconductive and chemically and thermally stable AEMs (and candidate alkalineionomers), as discussed below. AEMs in the hydroxide form typically becomebrittle if allowed to dry; hydroxide forms are typically prepared just before use,from the chloride form analogue.
14 R.C.T. Slade et al.Properties of AEMsThe most common class of NaOH-/KOH-free AEMs being investigated for use in fuelcells is based on QA chemistry and has reasonable stability in alkaline environments(especially those AEMs containing benzyltrimethyl ammonium exchange sites).There are three main classes of chemical degradation reaction mechanisms bywhich nucleophilic OHÀ anions can remove QA groups. The presence of b-hydrogensallows the Hofmann elimination reaction to occur (Scheme 2.1), often in parallelto the reactions discussed below, yielding alkene (vinyl) groups; this can give rise toQA–AEMs that have low thermal and chemical (to alkali) stabilities. If, as in RG-AEMs, no b-hydrogen atoms are present, direct nucleophilic substitution reactionswere traditionally thought to take place yielding alcohol and tertiary amine groups.However, recent density functional theory (DFT) calculations and deuterium ex-change experiments at Los Alamos National Laboratory (USA) on model small QA-containing compounds indicate that a mechanism involving an ylide intermediate(trimethyl ammonium methylide, also known as a 1,2-dipolar ylide compound) maypredominate and be more severe when the AEMs are dehydrated . H HO C H H H C N+Me2CH2 Me2NCH2 H H direct nucleophillic displacement mechanism + NMe3nucleophile OH- C C HO H H H N+Me3 H benzyltrimethylammonium cation Hβ Hβ + NMe3 + HOBβ N+Me3 Hβ C C Hα C C Hα Hα Hofmann elimination Hα mechanismScheme 2.1 Alternative mechanisms for degradation of AEMs by displacement of the trimethy-lammonium groups by hydroxide anions at elevated temperatures
2 Alkaline Membrane Fuel Cells 15 AEMs from Tokuyama Co have good thermochemical stability. The thin (10 mm)Tokuyama “fuel cell grade” AEMs (A010, A201 – formerly A006 and A901)[9, 36–39] and their developmental dispersible alkaline ionomers (A3ver.2 andAS–4) have also been tested at up to 50 C by several research groups in directalcohol fuel cells [40–42]. Quaternized pyridinium- or phosphonium-based AEMs were thought to havethermochemical stabilities that are not suitable for use in AEM fuel cells butthere are reports of recent work on polysulfone-phosphonium-based AEMs andanionomers (see later). Surrey’s benzyltrimethylammonium-containing S80, S50, and S20 RG–AEMs(the number designating the fully hydrated thicknesses in micrometers) are chemicallystable up to 80 C in aqueous KOH [32–34] (aq, 1 moldmÀ3) and can exhibit ionicconductivities 0.03 S cmÀ1 at room temperature when fully hydrated; the ex situ andin situ ionic conductivity of fully hydrated S80 is 0.06 S cmÀ1 at 60 C (cf. Naﬁon®acidic PEMs are typically 0.1 S cmÀ1 at these temperatures). AEM conductivitiesare, however, considerably reduced at humidities RH/% 100 and drop to valuesbetween 0.01 and 0.02 S cmÀ1 after only an hour when exposed to air (especially withvery thin membranes) due to the reaction of OHÀ anions with CO2 forming CO32À andHCO3À within the membrane. The lower dissociation constant for –NMe3OH groups(requiring a higher number of water molecules for complete dissociation), comparedto –SO3H groups in PEMs, and a very low number of water molecules directlyassociated with the ionic groups lead to the poor performance at low RHs (at highhumidities much of the water present in AEMs is located in aggregates not directlyassociated with the ionic groups) . The developing published and patent literature in this area has recently beenreviewed by Zeng and Varcoe . Further classes of AEM for fuel cells haveincluded membranes based on quaternized poly(epichlorohydrin), polysulfone,poly(phthalalazinone ether ketone), poly(2,6–dimethyl–1,4–phenylene oxide),and poly(vinyl alcohol) grafted with (2,3–epoxypropyl)trimethylammoniumchloride. Common quaternizing agents include alkyliodides, trialkylamines,N,N,N’,N’–tetramethylalkyl–1,n–diamines, polyethyleneimine, 1,4–diazabicy-clo–[2.2.2]–octane (DABCO), and 1–azabicyclo–[2.2.2]–octane. The ﬁnal twoof these have been used extensively; they contain b–hydrogen but their structuresdo not permit molecular conformations favored in the Hofmann eliminationmechanism. Metal-cation-containing AEMs based on doping polymer ﬁlms(e.g., polybenzimidazole (PBI), poly(vinyl alcohol) and its composites, and bio-compatible chitosan) with NaOH/KOH(aq) are also being investigated, but thepresence of mobile cations may introduce problems associated with precipitationof carbonate salts. Ionic conductivities of AEMs are generally lower than those of comparable PEMs.This is not surprising as the solution mobility of OHÀ is one third to one half of that ofa H+ (depending on the environment and if there – mo Â 104/cm2 VÀ1 sÀ1 = 20.64 forOHÀ(aq) anions and 36.23 for H+(aq) cations at 298 K) [1, 43]. One strategy forenhanced ionic conductivities is to increase the ion-exchange capacity (IEC) viasynthetic methodology, but this often leads to a decrease in the mechanical strength
16 R.C.T. Slade et al.due to excessive water uptakes. Another strategy is to synthesize tailored membranesthat will exhibit hydrophilic(ionic)–hydrophobic(nonionic) phase segregation andcontinuous ionic domains, which is hypothesized to increase ionic conductivities[44, 45]. Recent intensive studies have, however, been reported to lead to AEMs withhigh ionic conductivities, reportedly comparable to Naﬁon®. These promisingAEMs [11, 45–51] are still to be evaluated in AMFCs. Most hydrocarbon AEMsare soluble in various solvents, which is potentially useful for the formulation ofalkaline ionomers required for the preparation of high-performance membraneelectrode assemblies (MEAs). If the conductive properties reported can be translatedinto high power outputs, then AMFC performances comparable to those of PEMFCscan be expected in the near future.Synthetic Routes to AEMsThe preparation of applicable AEMs involves a compromise between the propertiesof the membrane, such as the chemical and thermal stability, ion-exchange capacity(IEC), ion conductivity, mechanical properties, water uptake, and dimensional stabil-ity. In general, alkaline anion-exchange polymer electrolytes can be polymerizeddirectly from functionalized monomers, polymerized from monomers with sub-sequent functionalization or by functionalizing a commercially available polymer.The backbone of the polymer is usually selected for its good chemical and thermalstability and, therefore, typically includes aromatic rings and/or a degree of ﬂuorina-tion: typical polymer classes include polysulfones and polyetherketones, polyimides,poly(phenylene), poly(phthalazinone ether sulfone ketone), polyepichlorohydrinhomopolymer, polybenzimidazole (PBI), poly(phenylene oxide), radiation-graftedcopolymers, inorganic–organic hybrids, and even perﬂuoronated membranes such asNaﬁon. The active functional groups are commonly quaternary ammonium type(ÀNR3+) with a clear preference for trimethylammonium (ÀN(CH3)3+) groups(pKa (H2O) = 9.8). A suitable AEM will have a high ion-exchange capacity, high ionic conductivity,and thermochemical stability, but will exhibit a low degree of swelling on hydration.There are several general synthetic methodologies for the preparation of AEMs[52, 53]. Fluorine-containing polymers generally show higher thermal stabilitiesthan hydrocarbon polymers. AEMs based on a poly(arylene ether sulfone) containingﬂuorine atoms show high ionic conductivities (63 mS cmÀ1 in CO32À form at 70 C); this is a key result as CO32À anions have dilute solution mobilities that areless than 33% of that of OHÀ anions. (It is rare to see CO32À conductivities above30 mS cmÀ1). Irradiation of polymer ﬁlms (and powders, etc.) using X-rays, g-rays, or electronbeams (as at Surrey, see previous section) is a ﬂexible way to introduce variousfunctional groups on the polymer backbones (Scheme 2.2). A wide range of
2 Alkaline Membrane Fuel Cells 17Scheme 2.2 The radiation-grafting of vinylbenzyl vinylbenzylchloride onto ETFE and chloridesubsequent amination andalkali-exchange, yieldingalkaline anion-exchangemembranes (RG-AEMs) CH2Cl ETFE ETFE electron beaming (CF2CF2-CH2CH2)n m CH2Cl 1) N(Me)3 (aq) ETFE 2) KOH (aq) m OH− CH2N+(Me)3chemically and thermal stable polymers, such as ETFE and FEP, can be chosen asthe base ﬁlms for the production of AEMs. Additionally, there is a wide choice offunctional monomers available that can be used to introduce ion-exchange groupsinto the grafted polymeric chains. A common strategy in the synthesis of AEMs is to introduce halogen alkylgroups onto the backbone or side chains of the polymer via chloroalkylation,ﬂuorination, bromination, or chlorination, followed by amination/quaternizationand ﬁnally ion exchange. Highly carcinogenic chloromethylethers have tradition-ally been used as the chloroalkylation agent but safer strategies have beenintroduced, for example, the chloro methylation agent is generated in situ (e.g.,[44, 55, 56]). An alternative strategy is the prior introduction of tertiary aminegroups into the polymer, followed by quaternization. The easiest synthetic route is to use inert polymers (as above) doped withconcentrated KOH(aq) (as above): polybenzimidazole (PBI) [57–61], poly(vinylalcohol) (PVA) , composite polymers such as PVA/hydroxyapatite (PVA/HAP), quaternized–PVA/alumina (QPVA/Al2O3) , PVA/titanium oxide (PVA/TiO2) [64, 65], chitosan and cross-linked chitosan [66–68], copolymers of epichlo-rohydrin and ethylene oxide , and cross-linked PVA/sulfosuccinic acid (10 wt.% SSA)  have all been doped with KOH and used as AEMs. Patent US5569559 describes the use of polar polymers (most preferred being polyethylene oxide)doped with alkaline metal hydroxides (such as KOH), alkaline earth metal
18 R.C.T. Slade et al.hydroxides or ammonium hydroxides such as tetrabutylammonium hydroxide; PBIdoped with KOH showed the highest ionic conductivity, comparable to Naﬁon® (astandard acidic proton-exchange membrane, PEM). All of these materials could,however, lead to carbonate precipitates. Anion-exchange polymers that contain methacrylate, ester, amide, or othercarbonyl (C = O double bond) functional groups show low stabilities in alkali asthese functional groups are highly reactive to nucleophiles such as OHÀ.Development of Alkaline IonomersAlkaline analogues to the oligomeric perﬂuorosulfonic acid dispersions used toproduce optimized ionic contact between the catalyst reaction sites and the PEMin PEMFCs have yet to be convincingly developed and this has resulted in the useof nonideal strategies for the fabrication of alkaline MEAs: the use of Naﬁondispersions (acidic, cation exchanging);concepts involving adsorbed potassiumhydroxide, and quaternized copolymers made from 4-vinylpyridine monomer atthe electrode–AEM interface. Polysulfone-based alkaline ionomers that are com-patible with polysulfone AEMs have been developed by various teams. On thecommercial front, it has been reported that Fumatech have developed a ionomerconcept for use with their commercial Fumasep®FAA AEMs, that uses twoprecursors that react to form a cross-linked polymer when mixed together, andTokuyama’s alkaline ionomers can be deposited from solution (designated A3 orAS-4) and are chemically compatible with Tokuyama’s fuel cell AEMs. Surrey developed an alkaline ionomer (SION1, Scheme 2.3) for MEA fabrica-tion, with the objective of developing a system that would allow the testing ofdifferent AEMs and electrodes in AMFCs ; without this alkaline ionomer, theperformances were too low for satisfactory testing. That alkaline ionomer alsoallowed for the operation of fuel cells in metal-cation-free mode, in contrast to thepossible use of doped polymers containing alkali metal hydroxides. An alkalineMEA that was deliberately converted to the CO32À form operated as well as an OHÀform MEA; even more interestingly, the CO32À content of the carbonated MEAdecreased during fuel cell operation with air (containing CO2) at the cathode. TheSION1 ionomer contains b–hydrogen atoms and, therefore, allows the Hofmannelimination degradation mechanism to operate, limiting the thermal stability tobelow ca. 60 C. Surrey is currently developing a next-generation b-hydrogen-freealkaline ionomers deposited from aqueous solutions (Patent GB 0814652.4). Many researchers have reported that alkaline polymers with hydrocarbonbackbones can be dissolved in solvents such as DMF, DMAc, and DMSO[47–49, 54, 73, 74], and this allows their use as the ionomer for the preparationof MEAs. Zhuang et al. [73, 75] used a quaternary ammonium polysulfone (QAPS)which can be dissolved in DMF and used as the ionomer; the QAPS polymer (inOHÀ form: IEC = 1.08 mmol gÀ1) was used to fabricate the membrane, whilea QAPS ﬁlm (OHÀ form: IEC = 1.18 meq gÀ1) was used as the ionomer.
2 Alkaline Membrane Fuel Cells 19Scheme 2.3 The formationof SION1 alkaline mionomer (anionomer) nby cross-linkage of poly a(vinylbenzyl chloride) withtetramethylhexanediamine Me2+N(TMHDA) OH− Me2+N CH2Cl OH− + Me2N OH− N+Me2 Cl NMe2 NMe2 p + KOH(aq) q + (H3C)2N-(CH2)6-N(CH3)2 n 2 CH2Cl + KOH exchange n n HO− -OH CH2 H2C (H3C)2N+−(CH2)6−N+(H3C)2 The development of alkaline ionomers is one of the major challenges for thedevelopment of high-performance alkaline membrane containing fuel cells. In state-of-the-art AMFC technology, the role of the ionomer has not been fully investigatedor understood; alkaline ionomer solutions/dispersions, comparable to the Naﬁondispersions used in PEMFCS, remain highly sought after.AMFCs with H2 as FuelFundamental studies at Surrey revealed the following [31–34]:A major source of performance loss is the mass transport of H2O to the ORR reactionsites. S80/S50/S20 radiation-grafted RG–AEMs, Solvay’s Morgane®–ADP, andTokuyama’s A201 were evaluated in H2/O2 fuel cells at Surrey using both commercial
20 R.C.T. Slade et al.Fig. 2.2 Variation in power 250density for H2/O2 AMFCs asa function of fully hydratedRG-AEM thickness. The cells 200 Power Density / mW cm−2contained ETFE-derived RG-AEMs. All electrodes weretreated with SION1 ionomer 150and utilized E-TekPt/C (20%mass) catalyst–loaded carboncloth (squares) or carbon 100paper (diamonds) supports 50 0 0 25 50 75 100 125 150 AAEM thickness / µm(prefabricated) and in-house produced electrodes containing SION1 ionomer . Asdiscussed earlier, water is required as a stoichiometric reactant for the ORR at thecathode when using AEMs (unlike in PEMFCs).The primary source of H2O to the cathode appears to be the back transport of theH2O electro-generated at the anode. Even with the use of fully hydrated gassupplies, evidence for this was that enhanced back transport of H2O from theanode, and therefore superior performances, was observed with thinner AEMs:beginning-of-life peak geometric power densities, Ppeak, of 54 ! 94 !130 mW cmÀ2 were recorded using 154 ! 78 ! 51 mm thick AEMs, respectively,under identical test conditions (less than 20 mW cmÀ2 was obtained with the230 mm thick Tokuyama AHA AEM – not developed for use in fuel cells)(Fig. 2.2). The commercial Pt/C (20% mass – 0.5 mgPt cmÀ2 loading)-containingType A carbon cloth prefabricated cathodes (E–Tek division of BASF) that wereused contained PTFE binder (current commercially available fuel cell electrodesare optimized for use with PEMs and not for AEMs) and it was suspected that thisrestricted the transport of the H2O supplied in the humidiﬁed oxygen supply to thereaction sites.Achieving an optimal MEA is still hindered by the available anionomers. Switchingto the use of Toray carbon paper commercial electrodes (435 mm thick containing Pt/C (20% mass) catalyst at 0.5 mgPt cmÀ2 loading and containing PTFE binder –supplied by E–Tek division of BASF) at both the anode and cathode led to anincrease in obtainable power densities (Fig. 2.2). Ppeak = 230 mW cmÀ2 anda maximum i at full discharge of 1.3 A cmÀ2 was obtained in a H2/O2 fuel cell at50 C with S20 (20 mm). A Ppeak = 260 mW cmÀ2 was obtained at 50 C withTokuyma A201 using SION1-treated electrodes. Fully satisfactory MEA laminationcannot, however, be achieved with SION1 alkaline ionomer and there are stillconsiderable, variable, contact resistances.
2 Alkaline Membrane Fuel Cells 21Pt-free electrodes are viable in AMFCs (more evidence is given below). Ag/C (60%mass, 4 mgAg cmÀ2) performed well when used as a cathode catalyst (Ag/C catalystperformed poorly in the cathode of a PEMFC). Open circuit voltages (VOC) werenormally in the range 1.0–1.1 V with Solvay ADP and Pt/C electrodes (ca. 100 mVhigher than obtained with Naﬁon–115 PEMFCs); a drop of 100 mV in VOC wasobserved when Pt was replaced with Ag at the cathode.The activity of the carbon supports needs to be evaluated for each catalyst material tobe tested. An important ﬁnding was that metal-free Vulcan XC–72R (i.e., carbonblack only) cathodes produced signiﬁcant currents (Ppeak = 22 mW cmÀ2 and VOC =0.88 V with Solvay ADP at 50 C). Carbons reduce O2 primarily through a 2eÀmechanism at high pH producing hydroperoxide anions (HO2À), which may formhighly reactive hydroxyl radical species. Other groups have been investigating nonradiation-grafted AEMs. A fully non-PGM-catalyst-containing metal-cation-free alkaline membrane fuel cell was ﬁrstreported by the team at Wuhan University , for an AMFC containing a QA-polysulfone AEM and an MEA that did not contain any PGM catalysts; a Ppeak =52 mW cmÀ2at 60 C (open circuit voltage, OCV, VOC = 0.94 V) was obtained usingNi-based anode catalyst and a Ag cathode catalyst. Polysulfone-based AEMs(see earlier) have been tested in H2/air fuel cells at 60 Cusing a polysulfone alkaline ionomer (dew point of the gases was 55 C). A Ppeak =28 mW cmÀ2 at Vcell = 0.47 V was obtained with Pt/C (40% mass, Johnson Matthey)with loadings of 0.5 mgPt cmÀ2. Ppeak = 30 mW cmÀ2 at Vcell = 0.42 V was obtainedwhen the cathode contained a Ag/C catalyst (40% mass, E–Tek) at a loading of2 mgAg cmÀ2. OCVs were 100 mV lower with Ag compared to Pt, which correlateswith the results above. A Ppeak = 365 mW cmÀ2 at 0.4 V (VOC = 1.04 V, r = 0.152Ω cm2) was reported at the 214th Meeting of the Electrochemical Society in 2008 byWang’s team at Penn State University, using Tokuyama’s A901 (10 mm) AEM andAS-4 alkaline ionomer (IEC = 1.3 meq gÀ1) at 50 C in a H2/O2 AMFC with0.4 mg cmÀ2Pt/C catalysts; these values dropped to 212 mW cmÀ2 (VOC = 1.02 V,r = 0.19 Ω cm2) when the O2 at the cathode was replaced with puriﬁed air (1 ppmCO2) and the Ppeak dropped to 113 mW cmÀ2 (r = 0.22 Ω cm2). The higher valuerepresents the highest H2/O2 AMFC performance publicly reported to date. KOH-doped membranes (see earlier) represent metal-cation-containing AEMs.A H2/O2 fuel cell has been tested with a KOH-doped PBI membrane (t = 40 mm) at50 C yielding an i = 620 mA cmÀ2 at Vcell = 0.60 V (P = 370 mW cmÀ2) . Thisperformance was similar to that of the same apparatus with a Naﬁon–117 PEM andalso, remarkably, with a PBI AEM doped with both KOH and K2CO3. The questionof the long-term stability and leaching out of the KOH (if any) remains to be fullyaddressed for this class of AEM, as does the issue of potential for carbonate/bicarbonate precipitation. Gu and Yan et al.  developed an ionomer, tris(2,4,6–trimethoxyphenyl)polysulfone–methylene quaternary phosphonium hydroxide (TPQPOH), which issoluble in low boiling point and water-soluble solvents such as methanol, ethanol,and n-propanol. The solubility of this kind of ionomer could be ideal for use in
22 R.C.T. Slade et al.AMFC MEAs; 196 mW cmÀ2 was achieved at 80 C (H2/O2 gases supplied at250 kPa back-pressure) using this phosphonium ionomer with a 70 mm thick FAAcommercial membrane (Fumatech GmbH) as the AEM. A maximum power ofmore than 250 mW cmÀ2 was obtained in a H2/O2 fuel cell at 50 C with a 50 mmAEM and gas back-pressures of 250 kPa. The presence of methoxy (ÀOCH3)groups on the aromatic rings that are connected to the phosphonium ion centersseems essential to adequate chemical stability.The Application of AEMs in Other Fuel Cell TypesThe utility of AEMs as potential electrolytes in fuel cells arises not only from theprospects for the use of non-Pt-group metal (non-PGM) catalysts and cheaper fuelcell components (less corrosive environment) but also from potential for use ofalternative fuels. Alcohols and diols, sodium borohydride (NaBH4), and hydrazine (H2NNH2) haveall been used directly as fuels in AMFCs. Patents [77, 78] introduced more fuelsincluding hydrated hydrazine (NH2NH2·H2O), hydrazine carbonate ((NH2NH2)2CO2),hydrazine sulfate (NH2NH2·H2SO4), monomethyl hydrazine (CH3NHNH2), ammonia(NH3), heterocycles such as imidazole and 1,3,5–truazine and 3–amino–1,2,4–triazole,and hydroxylamines such as hydroxylamine (NH2OH) and hydroxylamine sulfate(NH2OH·H2SO4); the catalysts were co-based for the fuel side (anode) and Ag/C, Pt/C and Ni/C for the oxygen reduction side (cathode). EP2133946  disclosed the useof transition metals as catalysts in AMFCs. There are numerous reports on the use ofnon-Pt catalyst, such as MnO2 , Ag/C [74, 75, 79], Au/C , FeTPP/BPC (BlackPearl Carbon) , CoPPyC , FeCo-CNF (Carbon Nanoﬁber) , CoFeN/C-HLH  in AMFC cathodes and Cr-decorated Ni/C , Fe-Co-Ni/C [85, 86] atanodes. Zhuang et al. conducted a feasibility analysis of the use of AEMs in DMFCs ;this important study concentrated on the thermodynamic disadvantages versuskinetic advantages of such cells by considering the reactions taking place in aqueoussolutions and the authors concluded that the thermodynamic voltage losses due tothe pH difference across the AEM would be approximately canceled out by thekinetic voltage gains. Ogumi et al. studied direct alcohol fuel cells (methanol andethylene glycol) with a commercial AEM (Tokoyama AHA, thickness % 240 mm). Solutions of ethylene glycol and methanol were made to a concentration of1 mol dmÀ3 dissolved in KOH (aq, 1 mol dmÀ3), and so the system was not metal-cation-free (common with other AMFCs obtaining reasonable power levels withalcohols as fuels). Cell voltages were around 100 mV higher for ethylene glycolcompared to methanol. This fuel cell is not quite an alkaline analogue of an acidmembrane DMFC, as the authors used alkaline fuel solution. No indication wasgiven concerning completeness of oxidation of the ethylene glycol to CO2 and H2O.Yu and Scott also reported the operation of a direct methanol alkaline fuel cell, with
2 Alkaline Membrane Fuel Cells 23platinized titanium mesh anodes (1.5 mg cmÀ2Pt/Ti) and a commercial alkalineanion-exchange membrane (Morgane ADP membrane from Solvay SA) . It has been proposed that ammonia would make a good energy vector/carrier and an indirect fuel for a hydrogen fuel cell; ammonia is environmentally benign (it isalready used as a fertilizer and neutralizes acid rain), already available cheaply,contains 50% more H per dm3 than liquid hydrogen, and is a liquid at much lowerpressures (8–9 bar); it also has the advantage of a strong smell, allowing the easierlocation of leaks. Cracking ammonia to form hydrogen free of traces of ammoniafor use in traditional PEMFCs requires temperatures of above 900 C; PEMFCscannot tolerate any NH3 contamination. An advantage of AFCs is that they willtolerate low levels of NH3, and so cracking can be undertaken at lower temperatures;this has yet to be explored using AMFC approaches.A Brief Overview of the Patent LiteratureZeng and Varcoe have recently reviewed in depth the patent literature concerningAEMs . A small number of patents of direct interest to application of AEMs inAMFCs are considered in this section. In the area of novel AEMs:• Patents relating to the application of radiation-grafted ion-exchange membranes in fuel cells have been granted to Scherer et al.  and to Stone and Steck [90, 91]. These patents mention the functionalization of base polymers with quaternary ammonium groups to yield alkaline polymers. The use of ﬂuorine-substituted styrenic monomers is also claimed to improve membrane chemical stability when utilized in fuel cells (removal of undesired and reactive C–H bonds).• Fauvarque was granted a patent on aqueous alkaline solid electrolyte based around polyether polymer matrices .• Yao et al. were granted related patents on alkaline polymers containing alkyl quaternary ammonium salts, nitrogen containing heterocyclic quaternary ammo- nium salts, and metal hydroxide salts for potential applications in alkaline batteries and fuel cells [93–95]. In the area of device architecture:• Jaouen patented a novel cathode structure for a solid polymer fuel cell ; that cathode structure consisted of a solid polymer anion-exchange membrane sur- rounding the catalysts particles (entirely within the cathode structure), which was in contact (surrounded) with a cation-conducting polymer membrane.• Lu and Zhuang were granted a patent on alkaline-resin-containing fuel cells with direct fuelling with liquid organic fuels .• Related patents from Divisek describe the invention of a methanol fuel cell utilizing an anion-exchange membrane [98, 99].
24 R.C.T. Slade et al.Future Directions and Research ChallengesThere are a number of research challenges that must be overcome before AEMs canbe successfully applied in pre-commercial AMFCs:1. As a priority and to complement ex situ stability measurements, AEMs must be evaluated in H2/O2, H2/air, and methanol/air fuel cells for several thousand hours to ensure adequate in situ membrane stability and assess the effect of and level of CO22À/HCO3À formation. The effect of adding alkali to the methanol solution must also be thoroughly investigated over long timescales.2. AEMs must be created with higher conductivities, to ensure good fuel cell performances at high current densities. It should be noted, however, that with application of an alkaline DMFC as a power source for portable devices, an overriding priority is maximizing the energy density of the fuel and fuel efﬁ- ciency (cell voltage). These DMFCs will be operated at low-to-medium current densities (higher efﬁciencies), where electrode overpotentials are the dominant cause of voltage losses.3. It is essential that a solubilized form of an alkaline anion-exchange polymer be developed to improve the interface between the electrodes and the AEM elec- trolyte. Success in this effort will decrease MEA resistances. A water-based soluble form which can be rendered water insoluble when cast would be preferred, as there are safety concerns (primarily with industrial scale produc- tion) about using organic solvents near ﬁnely dispersed (pyrophoric) metal catalysts (unsupported or supported on carbon).4. If AEMs are to be applied to fuel cells for other applications (such as automotive power etc.), more temperature stable AEMs must be developed. Operation of alkaline-membrane-based fuel cells at elevated temperature would reduce ther- modynamic voltage losses due to pH differences across the AEM and would also improve the electrokinetics. Successful, stable over the long term, and being operational at elevated temperatures, all would allow application in fuel cells for the automotive mass market.5. If AEMs are shown to be stable in fuel cells over thousands of hours, an in-depth investigation into effective and cheaper non-noble metal catalysts (e.g., Ni, Ag etc.) is indicated. There would also be a greater chance of ﬁnding methanol- tolerant catalysts for use in the cathodes than in related PEM-based DMFCs.6. Finally, removal of ﬂuorine from the polymer systems would be of interest to enhance the environmental credentials of the technology (facilitating easier disposal) and reduce costs. The substitution of fully ﬂuorinated FEP with non-ﬂuorinated LDPE is feasible. While oxidative radical degradation is a problem at the cathode and anode (via oxygen diffusion through the mem- brane) with non-ﬂuorinated PEMs, it has been shown using electron paramag- netic resonance (EPR) studies that such degradation is prevented in highly alkaline (pH 11.7) conditions pertinent to AEMs [100–102].
2 Alkaline Membrane Fuel Cells 25Acknowledgment We thank the Engineering and Physical Sciences Research Council (EPSRC)of the United Kingdom for contracts with our team in the area of development of alkalinemembrane technology for alkaline membrane fuel cells and associated electrical energy genera-tion: GR/S60709/01, EP/F027524/1, EP/G009929/2 and EP/H025340/1.BibliographyPrimary Literature 1. Varcoe JR, Slade RCT (2005) Prospects for alkaline anion-exchange membranes in low temperature fuel cells. Fuel Cells 5:189–200 2. Zeng R, Varcoe JR (2011) Alkaline anion exchange membranes for fuel cells – a patent review. Recent Pat Chem Eng 4:93–115 ¨ 3. Schulze M, Gulzow E (2004) Degradation of nickel anodes in alkaline fuel cells. J Power Sources 127:252–263 ¨ 4. Wagner N, Schulze M, Gulzow E (2004) Long term investigations of silver cathodes for alkaline fuel cells. J Power Sources 127:264–272 5. McLean GF, Niet T, Prince-Richard S, Djilali N (2002) An assessment of alkaline fuel cell technology. Int J Hydrogen Energy 27:507–526 6. Cifrain M, Kordesch KV (2004) Advances, aging mechanism and lifetime in AFCs with circulating electrolytes. J Power Sources 127:234–242 ¨ 7. Gulzow E, Schulze M (2004) Long-term operation of AFC electrodes with CO2 containing gases. J Power Sources 127:243–251 8. Zeng R, Poynton SD, Kizewski JP, Slade RCT, Varcoe JR (2010) A novel reference electrode for application in alkaline polymer electrolyte membrane fuel cells. Electrochem Commun 12:823–8355 9. Yanagi H, Fukuta K (2008) Anion exchange membrane and ionomer for alkaline membrane fuel cells (AMFCs). Electrochem Soc Trans 16:257–262 10. Kizewski JP, Mudri NH, Zeng R, Poynton SD, Slade RCT, Varcoe JR (2010) Alkaline electrolytes and reference electrodes for alkaline polymer electrolyte membrane fuel cells. Electrochem Soc Trans 33:27–35 11. Yan JL, Hickner MA (2010) Anion exchange membranes by bromination of benzylmethyl–- containing poly(sulfone)s. Macromolecules 43:2349–2356 12. Adams LA, Poynton SD, Tamain C, Slade RCT, Varcoe JR (2008) A carbon dioxide tolerant aqueous–electrolyte–free anion–exchange membrane alkaline fuel cell. Chem Sus Chem 1:79–81 13. Zagorodni AA, Kotova DL, Selemenev VF (2002) Infrared spectroscopy of ion exchange resins: chemical deterioration of the resins. React Funct Polym 53:157–171 14. Neagu V, Bunia I, Plesca I (2000) Ionic polymers – VI. Chemical stability of strong base anion exchangers in aggressive media. Polym Degrad Stab 70:463–468 15. Sata T, Tsujimoto M, Yamaguchi T, Matsusaki K (1996) Change of anion exchange membranes in an aqueous sodium hydroxide solution at high temperature. J Membr Sci 112:161–170 16. Soda T, Kaisha K (1972) Anion exchange membranes and their production. GB Patent 1401997 17. Hansen RD, Wheaton RM (1966) Separation of acid from polymers by dialysis with anion exchange membrane. US Patent 3244620
26 R.C.T. Slade et al. 18. Imoto R, Kosaka Y, Shimizu A (1966) Process for manufacturing anion-exchange membranes from a graft copoloymer of SBR and a vinylpyridine reacted with an epoxy resin. US Patent 3258435 19. Hansen RD, Wheaton RM (1966) Separation of acid by dialysis with anion-exchange membranes. US Patent 3272737 ¨ 20. Suser A (1973) Preparation of anion exchange membranes from cellulose sheets. US Patent 3714010 21. Scott, Rosedale, Moulton, Taylor, Gough (1990) Anion exchange membranes. Patent EP0382439 22. Altmeier P (1995) Stark basische anionenaustauschermembranen und verfahren zu deren herstellung. Patent WO9506083 23. Altmeier P (1998) Strongly alkaline anion exchange membranes and process for producing the same. US Patent 5746917 24. Ehrikhovich KJ, Viktorovna SN, Aleksandrovich FJ, Semenovich GS, Mikhajlovich AJ, Vladimirovna SI, Alekseevna JN, Fedorovich TS (1997) Method for production of anion- exchange membranes having high penetrability to chloride ion. Patent RU2074204 25. Jurevich TD (2007) Method for modifying anion-exchange membranes MA-40. Patent RU2303835 26. Aminabhavi T, Kulkarni PV, Kariduraganavar MY (2009) Ion exchange membranes, methods and processes for production thereof and uses in speciﬁc applications. US Patent 7544278 27. Danks TN, Slade RCT, Varcoe JR (2002) Comparison of PVDF– and FEP–based radiation–grafted alkaline anion–exchange membranes for use in low temperature portable DMFCs. J Mater Chem 12:3371–3373 28. Danks TN, Slade RCT, Varcoe JR (2003) Alkaline anion–exchange radiation–grafted membranes for possible electrochemical application in fuel cells. J Mater Chem 13:712–721 29. Herman H, Slade RCT, Varcoe JR (2003) The radiation–grafting of vinylbenzyl chloride onto poly(hexaﬂuoropropylene–co–tetraﬂuoroethylene) ﬁlms with subsequent conversion to alkaline anion–exchange membranes: optimisation of the experimental conditions and char- acterization. J Membr Sci 218:147–163 30. Tzanetakis N, Varcoe J, Slade RS, Scott K (2003) Salt splitting with radiation grafted PVDF anion–exchange membrane. Electrochem Commun 5:115–119 31. Tzanetakis N, Varcoe JR, Slade RCT, Scott K (2005) Radiation–grafted PVDF anion exchange membrane for salt splitting. Desalination 174:257–265 32. Slade RCT, Varcoe JR (2005) Investigations of conductivity in FEP–based radiation–grafted alkaline anion–exchange membranes. Solid State Ionics 176:585–597 33. Varcoe JR, Slade RCT (2006) An electron–beam–grafted ETFE alkaline anion–exchange membrane in metal–cation–free solid–state alkaline fuel cells. Electrochem Commun 8:839–843 34. Varcoe JR, Slade RCT, Yee ELH, Poynton SD, Driscoll DJ, Apperley DC (2007) Poly (ethylene–co–tetraﬂuoroethylene)–derived radiation–grafted anion–exchange membrane with properties speciﬁcally tailored for application in metal–cation–free alkaline polymer electrolyte fuel cells. Chem Mater 19:2686–2693 35. Chempath S, Einsla BR, Pratt LR, Macomber CS, Boncella JM, Rau JA, Pivovar BS (2008) Mechanism of tetra alkyl ammonium head group degradation in alkaline fuel cell membranes. J Phys Chem C 112:3179–3182 36. Piana M, Boccia M, Filpi A, Flammia E, Miller HA, Orsini M, Salusti F, Santiccioloi S, Ciardelli F, Pucci A (2010) H2/air alkaline membrane fuel cell performance and durability, using novel ionomer and non–platinum group metal cathode catalyst. J Power Sources 195:5875–5881 37. Li YS, Zhao TS, Liang ZX (2009) Performance of alkaline electrolyte–membrane–based direct ethanol fuel cells. J Power Sources 187:387–392
2 Alkaline Membrane Fuel Cells 27 38. Kim JH, Kim HK, Hwang KT, Lee JY (2010) Performance of air–breathing direct methanol fuel cell with anion–exchange membrane. Int J Hydrogen Energy 35:768–773 39. Matsuoka K, Iriyama Y, Abe T, Matsuoka M, Ogumi Z (2005) Alkaline direct alcohol fuel cells using an anion exchange membrane. J Power Sources 150:27–31 40. Li YS, Zhao TS, Liang ZX (2009) Effect of polymer binders in anode catalyst layer on performance of alkaline direct ethanol fuel cells. J Power Sources 190:223–229 41. Fujiwara N, Siroma Z, Yamazaki SI, Ioroi T, Senoh H, Yasuda K (2008) Direct ethanol fuel cells using an anion exchange membrane. J Power Sources 185:621–626 42. Bunazawa H, Yamazaki Y (2008) Inﬂuence of anion ionomer content and silver cathode catalyst on the performance of alkaline membrane electrode assemblies (MEAs) for direct methanol fuel cells (DMFCs). J Power Sources 182:48–51 43. Marx D, Chandra A, Tuckerman ME (2010) Aqueous basic solutions: hydroxide solvation, structural diffusion, and comparison to the hydrated proton. Chem Rev 110:2174–2216 44. Hibbs MR, Hickner MA, Alam TM, McIntyre SK, Fujimoto CH, Cornelius CJ (2008) Trans- port properties of hydroxide and proton conducting membranes. Chem Mater 20:2566–2573 45. Robertson NJ, Kostalik HA IV, Clark TJ, Mutolo PF, Abruna HD, Coates GW (2010) Tunable high performance cross–linked alkaline anion exchange membranes for fuel cell applications. J Am Chem Soc 132:3400–3404 46. Tanaka M, Koike M, Miyatake K, Watanabe M (2010) Anion conductive aromatic ionomers containing ﬂuorenyl groups. Macromolecules 43:2657–2659 47. Wang JH, Li SH, Zhang SB (2010) Novel hydroxide–conducting polyelectrolyte composed of a poly(arylene ether sulfone) containing pendant quaternary guanidinium groups for alkaline fuel cell applications. Macromolecules 43:3890–3896 48. Guo ML, Fang J, Xu HK, Li W, Lu XH, Lan CH, Li KY (2010) Synthesis and characteriza- tion of novel anion exchange membranes based on imidazolium–type ionic liquid for alkaline fuel cells. J Membr Sci 362:97–104 49. Wang JH, Zhao Z, Gong FX, Li SH, Zhang SB (2009) Synthesis of soluble poly(arylene ether sulfone) ionomers with pendant quaternary ammonium groups for anion exchange membranes. Macromolecules 42:8711–8717 50. Tripathi BP, Kumar M, Shahi VK (2010) Organic–inorganic hybrid alkaline membranes by epoxide ring opening for direct methanol fuel cell applications. J Membr Sci 360:90–101 51. Clark TJ, Robertson NJ, Kostalik HA IV, Lobkovsky EB, Mutolo PF, Abruna HD, Coates GW (2009) A ring–opening metathesis polymerization route to alkaline anion exchange membranes: development of hydroxide–conducting thin ﬁlms from an ammonium–- functionalized monomer. J Am Chem Soc 131:12888–12889 52. Shevchenko VV, Gumennaya MA (2010) Synthesis and properties of anion-exchange membranes for fuel cells. Theor Exp Chem 46:139–152 53. Varcoe JR, Poynton SD, Slade RCT (2009) In: Vielstich W, Gasteiger HA, Yokokawa H (eds) Handbook of fuel cells – fundamentals, technology and applications, vol 5, Advances in electocatalysis, materials, diagnostics and durability. Wiley, Chichester, pp 322–336 54. Zhou J, Unlu M, Vega J, Kohl P (2009) Anionic polysulfoneionomers and membranes containing ﬂuorenyl groups for anionic fuel cells. J Power Sources 190:285–292 55. Fang J, Shen PK (2006) Quaternizedpoly(phthalazinon ether sulfone ketone) membrane for anion exchange membrane fuel cells. J Membr Sci 285:317–322 56. Zeng QH, Liu QL, Broadwell I, Zhu AM, Xiong Y, Tu XP (2010) Anion exchange membranes based onquaternized polystyrene–block–poly(ethylene–ran–butylene)–block–polystyrene for direct methanol alkaline fuel cells. J Membr Sci 349:237–243 57. Hou HY, Sun GQ, He RH, Wu ZM, Sun BY (2008) Alkali doped polybenzimidazole membrane for high performance alkaline direct ethanol fuel cell. J Power Sources 182:95–99 58. Hou HY, Sun GQ, He RH, Sun BY, Jin W, Liu H, Xin Q (2008) Alkali doped polybenzi- midazole membrane for alkaline direct methanol fuel cell. Int J Hydrogen Energy 33:7172–7176
28 R.C.T. Slade et al. 59. Modestov AD, Tarasevich MR, Leykin AY, Filimonov VY (2009) MEA for alkaline direct ethanol fuel cell with alkali doped PBI membrane and non–platinum electrodes. J Power Sources 188:502–506 60. Xing B, Savadogo O (2000) Hydrogen oxygen polymer electrolyte membrane fuel cells (PEMFCs) based on alkaline–doped polybenzimidazole (PBI). Electrochem Commun 2:697–702 61. Savadogo O (2004) Emerging membranes for electrochemical systems. Part II. High temper- ature composite membranes for polymer electrolyte fuel cell (PEFC) applications. J Power Sources 127:135–161 62. Yang CC, Lin CT, Chiu SJ (2008) Preparation of the PVA/HAP composite polymer mem- brane for alkaline DMFC application. Desalination 233:137–146 63. Yang CC, Chiu SJ, Chien WC, Chiu SS (2010) Quaternized poly(vinyl alcohol)/alumina composite polymer membranes for alkaline direct methanol fuel cells. J Power Sources 195:2212–2219 64. Yang CC, Chiu SJ, Lee KT, Chien WC, Lin CT, Huang CA (2008) Study of poly(vinyl alcohol)/titanium oxide composite polymer membranes and their application on alkaline direct alcohol fuel cell. J Power Sources 184:44–51 65. Yang CC (2007) Synthesis and characterization of the cross–linked PVA/TiO2 composite polymer membrane for alkaline DMFC. J Membr Sci 288:51–60 66. Wan Y, Peppley B, Creber KAM, Bui VT, Halliop E (2006) Preliminary evaluation of an alkaline chitosan–based membrane fuel cell. J Power Sources 162:105–113 67. Wan Y, Creber KAM, Peppley B, Bui VT (2006) Chitosan–based electrolyte composite membranes II. Mechanical properties and ionic conductivity. J Membr Sci 284:331–338 68. Wan Y, Creber KAM, Peppley B, Bui VT (2006) Chitosan–based solid electrolyte composite membranes I. Preparation and characterization. J Membr Sci 280:666–674 69. Vassal N, Salmon E, Fauvarque JF (2000) Electrochemical properties of an alkaline solid polymer electrolyte based on P(ECH–co–EO). Electrochim Acta 45:1527–1532 70. Yang CC, Chiu SJ, Chien WC (2006) Development of alkaline direct methanol fuel cells based on cross–linked PVA polymer membranes. J Power Sources 162:21–29 71. Fauvarque JF (1996) Alkaline solid polymer electrolyte, electrode and electrochemical generator containing such as electrolyte. US Patent 5569559 72. Varcoe JR, Slade RCT, Lam How Yee E (2006) An alkaline polymer electrochemical interface: a breakthrough in application of alkaline anion–exchange membranes in fuel cells. Chem Commun :1428–29 73. Lu SF, Pan J, Huang AB, Zhuang L, Lu JT (2008) Alkaline polymer electrolyte fuel cells completely free from noble metal catalysts. Proc Natl Acad Sci 105:20611–20614 74. Park JS, Park SH, Yim SD, Yoon YG, Lee WY, Kim CS (2008) Performance of solid alkaline fuel cells employing anion–exchange membranes. J Power Sources 178:620–626 75. Tang DP, Pan J, Lu SF, Zhuang L, Lu JT (2010) Alkaline polymer electrolyte fuel cells: principle, challenges, and recent progress. Sci China Chem 53:357–364 76. Gu S, Cai R, Luo T, Chen ZW, Sun MW, Liu Y, He GH, Yan YS (2009) A soluble and highly conductive ionomer for high–performance hydroxide exchange membrane fuel cells. Angew Chem Int Ed 48:6499–6502 77. Asazawa K, Yamada K, Tanaka H (2007) Fuel cell. Patent EP1843416 78. Tanaka H, Yamada K, Asazawa K (2004) Fuel cell. Patent EP1460705 79. Asazawa K, Yamada K, Tanaka H (2009) Fuel cell. Patent EP2133946 80. Poynton SD, Kizewski JP, Slade RCT, Varcoe JR (2010) Novel electrolyte membranes and non–Pt catalysts for low temperature fuel cells. Solid State Ionics 181:219–222 81. Ramaswamy N, Mukerjee S (2010) Electrocatalysis of oxygen reduction on non-precious metallic centers at high pH environments. ECS Trans 33:1777–1785 82. Asazawa K, Yamamoto K, Yamada K, Tanaka H, Matsumura D, Tamura K, Nishihata Y, Atanassov P (2010) XAFS analysis of unpyrolyzedCoPPyC oxygen reduction catalyst for anion-exchange membrane fuel cells (AMFC). Electrochem Soc Trans 33:1751–1755
2 Alkaline Membrane Fuel Cells 29 83. Jeong B, Uhm S, Lee J (2010) Iron-cobalt modiﬁed electrospun carbon nanoﬁbers as oxygen reduction catalysts in alkaline fuel cells. Electrochem Soc Trans 33:1757–1767 84. Li XG, Popov BN, Kawahara T, Yanagi H (2010) Recent advances in non-precious metal catalysts for oxygen reduction reaction in fuel cells. Electrochem Soc Trans 33:1769–1776 85. Takeguchi T, Takahashi H, Yamanaka T, Nakamura A, Ueda W (2010) Development of direct-ethanol anion-conducting solid alkaline inorganic fuel cell. Electrochem Soc Trans 33:1847–1851 86. Nakamura A, Takahashi H, Takeguchi T, Yamanaka T, Wang Q, Uchimoto Y, Ueda W (2010) Effect of reduction temperature of Fe-Co-Ni/C catalyst on the solid alkaline fuel cell performance. Electrochem Soc Trans 33:1817–1821 87. Wang Y, Li L, Hu L, Zhuang L, Lu J, Xu B (2003) A feasibility analysis for alkaline membrane direct methanol fuel cell: thermodynamic disadvantages versus kinetic advantages. Electrochem Commun 5:662–666 88. Yu EH, Krewer U, Scott K (2010) Principles and materials aspects of direct alkaline alcohol fuel cells. Energies 3:1499–1528 ¨ 89. Scherer GG, Buchi FN, Gupta G (Paul Scherrer Institut, Switzerland) (1997) US Patent 5656386 90. Stone C, Steck A (Ballard Power Systems Inc., Canada) (2002) US Patent 6359019 91. Stone C, Steck A (Ballard Power Systems Inc., Canada) (2000) PCT Patent 01/58576 ´ 92. Fauvarque J-F (CNAM Paris and Electricite de France) (1996) US Patent 5569559 93. Yao W, Tsai T, Chang Y-M, Chen M (Reveo Inc., USA) (2001) US Patent 6183914 94. Yao W, Tsai T, Chang Y-M, Chen M (Reveo Inc., USA) (2000) PCT Patent 00/16422 95. Yao W, Tsai T, Chang Y-M, Chen M (Reveo Inc., USA) (2000) Patent EP1116291 96. Jaouen F (ABB AB and Volvo, Sweden) (2002) PCT Patent 02/35633 97. Lu J, Zhuang L (Wuhan University) (2003) Patent CN1402370 ¨ 98. Divisek J (Forschungszentrum Julich, Germany) (2001) PCT Patent 01/61776 ¨ 99. Divisek J (Forschungszentrum Julich, Germany) (2001) Patent EP1256142100. Yu J, Yi B, Xing D, Liu F, Shao Z, Fu Y, Zhang H (2003) Degradation mechanism of polystyrene sulfonic acid membrane and application of its composite membranes in fuel cells. Phys Chem Chem Phys 5:611–615101. Hubner G, Roduner E (1999) EPR investigation of HQ radical initiated degradation reactions ¨ of sulfonated aromatics as model compounds for fuel cell proton conducting membranes. J Mater Chem 9:409–418 ¨102. Panchenko A, Dilger H, Moller E, Sixt T, Roduner E (2004) In situ EPR investigation of polymer electrolyte membrane degradation in fuel cell applications. J Power Sources 127:325–330